Table 19. Continued. 













Corrosion 







Alloy 



CDA 

 No. a 



Environment 



Exposure 

 (day) 



Depth 



(ft) 



Rate 



(mpy) 



Type of 

 Corrosion* 7 



Source 



Ni-Al Bronze No. 2 



_ 



W 



123 



5,640 



0.5 



U 



INCO (3) 



Ni-Al Bronze No. 2 



- 



S 



123 



5,640 



0.3 



u 



INCO (3) 



Ni-Al Bronze No. 2 



- 



W 



403 



6,780 



0.2 



I-p 



INCO (3) 



Ni-Al Bronze No. 2 



- 



S 



403 



6,780 



0.1 



u 



INCO (3) 



Ni-Al Bronze No. 2 



- 



w 



751 



5,640 



0.5 



SL-DA 



INCO (3) 



Ni-Al Bronze No. 2 



- 



S 



751 



5,640 



0.2 



C(13) 



INCO (3) 



Ni-Al Bronze No. 2 



- 



w 



1,064 



5,300 



0.2 



C(5) 



INCO (3) 



Ni-Al Bronze No. 2 



- 



s 



1,064 



5,300 



0.5 



CR(21) 



INCO (3) 



Ni-Al Bronze No. 2 



- 



w 



197 



2,340 



0.3 



U 



INCO (3) 



Ni-Al Bronze No. 2 



- 



s 



197 



2,340 



0.1 



U 



INCO (3) 



Ni-Al Bronze No. 2 



- 



w 



402 



2,370 



0.2 



U 



INCO (3) 



Ni-Al Bronze No. 2 



- 



s 



402 



2,370 



<0.1 



ET 



INCO (3) 



Ni-Al Bronze No. 2 



- 



w 



181 



5 



1.0 



C(8) 



INCO (3) 



Ni-Al Bronze No. 2 



- 



w 



366 



5 



0.4 



U 



INCO (3) 



Ni-Al Bronze No. 3 



- 



w 



123 



5,640 



0.4 



U 



INCO (3) 



Ni-Al Bronze No. 3 



- 



s 



123 



5,640 



0.3 



U 



INCO (3) 



Ni-Al Bronze No. 3 



- 



w 



403 



6,780 



0.2 



u 



INCO (3) 



Ni-Al Bronze No. 3 



- 



s 



403 



6,780 



<0.1 



NU-ET 



INCO (3) 



Ni-Al Bronze No. 3 



- 



w 



751 



5,640 



0.2 



I-P 



INCO (3) 



Ni-Al Bronze No. 3 



- 



s 



751 



5,640 



0.1 



U 



INCO (3) 



Ni-Al Bronze No. 3 



- 



w 



1,064 



5,300 



<0.1 



P(4) 



INCO (3) 



Ni-Al Bronze No. 3 



- 



s 



1,064 



5,300 



0.2 



CR(10) 



INCO (3) 



Ni-Al Bronze No. 3 



- 



w 



197 



2,340 



0.3 



U 



INCO (3) 



Ni-Al Bronze No. 3 



" 



s 



197 



2,340 



0.2 



U 



INCO (3) 



Si Bronze, 3% 



65 3 



w 



123 



5,640 



1.3 



U 



INCO (3) 



Si Bronze, 3% 



653 



s 



123 



5,640 



1.5 



U 



INCO (3) 



Si Bronze, 3% 



65 3 



w 



403 



6,780 



1.2 



MO-CO 



INCO (3) 



Si Bronze, 3% 



65 3 



s 



403 



6,780 



0.4 



GBSL 



INCO (3) 



Si Bronze, 3% 



653 



w 



751 



5,640 



1.0 



U 



INCO (3) 



Si Bronze, 3% 



653 



s 



751 



5,640 



0.7 



U 



INCO (3) 



Si Bronze, 3% 



65 3 



w 



1,064 



5,300 



0.6 



MO-CO 



INCO (3) 



Si Bronze, 3% 



65 3 



s 



1,064 



5,300 



0.4 



SL-CO 



INCO (3) 



Si Bronze, 3% 



653 



w 



197 



2,340 



1.1 



u 



INCO (3) 



Si Bronze, 3% 



653 



s 



197 



2,340 



0.1 



NU-ET 



INCO (3) 



Si Bronze, 3% 



653 



w 



402 



2,370 



1.2 



U 



INCO (3) 



Si Bronze, 3% 



653 



s 



402 



2,370 



0.2 



ET 



INCO (3) 



Si Bronze, 3% 



653 



w 



181 



5 



1.7 



U 



INCO (3) 



Si Bronze, 3% 



653 



w 



366 



5 



1.1 



G 



INCO (3) 



Si Bronze A 



655 



w 



123 



5,640 



1.6 



U 



CEL (4) 



Si Bronze A 



655 



w 



123 



5,640 



1.4 



U 



INCO (3) 



Si Bronze A 



655 



s 



123 



5,640 



1.8 



u 



CEL (4) 



Si Bronze A 



655 



s 



123 



5,640 



1.5 



u 



INCO (3) 



Si Bronze A 



655 



w 



403 



6,780 



1.2 



CO 



CEL (4) 



Si Bronze A 



655 



w 



403 



6,780 



1.2 



u 



INCO (3) 



Si Bronze A 



655 



s 



403 



6,780 



1.8 



ET 



CEL (4) 



Si Bronze A 



655 



s 



403 



6,780 



0.2 



GBSL 



INCO (3) 



Si Bronze A 



655 



w 



751 



5,640 



0.8 



S-CO 



CEL (4) 



Si Bronze A 



655 



w 



751 



5,640 



1.4 



U 



INCO (3) 



Si Bronze A 



655 



s 



751 



5,640 



0.9 



G 



INCO (3) 



75 



